Fundamentals of grain boundaries and grain boundary migration


 Donald Cobb
 3 years ago
 Views:
Transcription
1 1. Fundamentals of grain boundaries and grain boundary migration 1.1. Introduction The properties of crystalline metallic materials are determined by their deviation from a perfect crystal lattice, which occurs due to their intrinsic crystal defects. Without those crystal defects, metals would never have been used in such a wide variety of applications []. There are different types of crystal defects which are distinguished by their spatial dimension. One of the longest known and most important defects in metals is the grain boundary, a twodimensional planar defect, which separates two adjacent crystallites of the same crystal structure and chemical composition, but of different orientation [1]. Since any crystalline material, except for single crystals, is granularstructured, grain boundaries are the fundamental defect in polycrystalline materials, exerting a substantial impact on their properties []. 1.. Classification In threedimensional space, there are eight degrees of freedom, which means eight independent parameters are required to assign a mathematically exact definition to a given grain boundary [9]. Three parameters are necessary to define the orientation relationship between two adjacent grains which are usually represented by an Euler angle triplet ( 1,, ), by Miller indices or by an angleaxis pair in RodriguesFrank space [, 3, 4]. Two more parameters are needed to define the spatial orientation of the grain boundary plane, i.e. the boundary inclination, which are expressed by the normalized crystallographic normal vector of the plane of inclination n = (n 1, n, 4
2 n 3 ) with respect to one of the adjacent grains. Additional to these five macroscopic parameters there are three independent values of the microscopic translational vector t = (t 1, t, t 3 ) []. All intrinsic properties of grain boundaries, particularly mobility and energy, are functions of these eight parameters [1]. The five macroscopic parameters may be influenced externally, whereas the translational vector t is determined by the minimum of the total energy of the crystal. To determine the dependence of grain boundary properties on the five macroscopic parameters introduced above, it would be necessary to keep all but one degree of freedom constant and successively vary one free parameter [1, ]. However, under realistic experimental conditions only one set of parameters may remain at a fixed value. The most common investigation procedure therefore is to change an orientation relationship by varying the rotation angle and keeping the plane of inclination fixed with respect to a reference point or vice versa while preserving one common axis of rotation [1] Presentation of misorientations The misorientation or orientation relationship between two differently oriented crystallites is a spatial transformation applied to one crystal in order to bring both orientations to coincidence [1]. Assuming a common origin for both lattices, this is achieved by a simple rotation of one lattice relative to the other, which is conveniently expressed by a rotation transformation matrix m g : 5
3 m g C C (1.1) i j where i C and C are the crystal coordinate systems. The easiest way to j describe such a rotation matrix is in terms of a rotation axis <hkl> common for both lattice coordinate systems and a rotation angle (Fig. 11), since for many z z uvtw x x y y Fig. 11: Rotation about axis <uvtw> of angle brings coordinate system 1 and to coincide. cases it is of major interest to investigate the influence of the rotation angle on a grain boundary property for a certain rotation axis [1]. Thus, it is common to keep the grain boundary inclination constant and only take into account the rotation angle dependence. Consequently, grain boundaries may be divided into three different categories. In case of a rotation axis perpendicular to the grain boundary plane, the grain boundary is given the denotation twist boundary (Fig. 1 a). For this type of grain boundary the grain boundary plane is exactly defined and independent of the rotation angle. In Figures 1 b and 1 c the class of tilt grain boundaries is depicted. The major difference to twist 6
4 boundaries is that the rotation axis is aligned parallel to the boundary plane [1]. Consequently, an infinite number of possible grain boundary planes exists for a given rotation angle. Further, one distinguishes between two types of grain boundary within the class of tilt boundaries. Under the special conditions that mirror symmetry is satisfied between two adjacent grains, the boundary is labeled as a symmetrical tilt boundary (Fig. 1 c). All other configurations are denoted as asymmetrical tilt boundaries (Fig. 1 b) [1]. rotation axis (a) grain boundary (b) symmetry plane [uvtw] 1 [uvtw] grain boundary tilt axis and grain boundary (c) boundary plane rotation axis Fig. 1: Schematic depictions of a) a twist grain boundary and b) an asymmetrical tilt and c) a symmetrical tilt boundary [1] Grain boundaries that do not satisfy either of the criteria of the first two classes are termed mixed or random grain boundaries and consist of both twist and tilt components. 7
5 1.4. Atomic structure An additional means to classify grain boundaries is to categorize them, depending on their misorientation, by distinguishing between low angle grain boundaries (LAGBs) and high angle boundaries (HAGBs). In the following sections the difference between these grain boundaries regarding their microstructural configuration will be addressed Low angle grain boundaries Providing the case that the misorientation angle between two neighboring grains is small enough (LAGB), the misorientation of the grain boundary is achieved by lattice distortions introduced by dislocation arrays. In case of a symmetrical 1010 tilt boundary, the configuration consists of a single set of edge dislocations with Burgers vectors b, where the dislocation spacing directly correlates with the misorientation angle (Fig. 13a) [1]. b d sin (.1) Accompanied with an increasing misorientation angle the spacing d decreases as depicted in Fig
6 boundary 6 b grain 1 d = b/ grain dislocation spacing d [104 cm] measured d = (a) (b) tilt angle [104 rad] Fig. 13: a) Schematic depiction of a symmetrical low angle tilt boundary, b) measured and calculated dislocation spacing versus tilt angle in a symmetrical LAGB in Germanium [1] For asymmetrical tilt grain boundaries (Fig. 1 b), in which the boundary plane deviates from its symmetrical position by an inclination angle (Fig. 14), at least two sets of edge dislocations are necessary to accommodate the boundary configuration. The Burgers vector of these two dislocation sets must be perpendicular to each other (Fig. 14 a) and with increasing asymmetry, the fraction of the second set of dislocations ( b ) has to increase, 1 d sin (.) b while the fraction of dislocations with Burgers vector b 1 decreases with. 9
7 a) b) uvtw1 1/ / plane of symmetry / 1/ uvtw boundary plane Fig. 14: a) Lattice dislocation arrangement [1] and b) rotation angle and inclination angle of an asymmetrical tilt LAGB. 1 1 d (.3) cos 1 b Small angle twist boundaries require two sets of screw dislocations and in the most general case of mixed LAGBs the boundary structure is comprised of dislocation networks of three Burgers vectors [5]. By applying this dislocation model of LAGBs, which was developed by Read and Shockley [6], the exact calculation of free grain boundary energy is possible. As derived by Read and Shockley, the stress field of dislocations in an infinite periodic array is spatially limited to a range of the order of spacing d. In case of an edge dislocation its energy E d per unit length is thus expressed by: 10
8 E b d 4 1 r E c 0 ln d (.4) where is the Poisson ratio, the shear modulus, r0 b the radius and E c the energy of the dislocation core [1]. Keeping in mind, that this equation needs to be applied to a set of dislocations, which compose a LAGB, we introduce the number of dislocations per unit length n 1/ d / bto the above equation and thereby obtain the energy per unit area for the case of a symmetrical tilt grain boundary: symm b b 1 ln E A B ln b c 4 (1 ) (.5) where A Ec / b and B b / 4 (1 ). Comparing the energies obtained by calculation with equation.4 to experimental data [7] proves the validity of this dislocation model, as the energy increase with increasing angle of rotation is predicted, accordingly, for angles 15 [1] High angle grain boundaries For rotation angles larger than 15, the lattice dislocation model no longer applies, as the dislocation cores are brought to an overlapping [8], causing the loss of their identity as individual lattice defects. Therefore, grain boundaries with rotation angles larger than 15 are distinguished from LAGBs and are 11
9 termed high angle grain boundaries (HAGB). The current concept of the structure of HAGBs was deduced from geometrical considerations, based on dislocation models for LAGBs and atomistic simulations [5, 7, 9, 1]. Most commonly, the structure of interfaces is described by the coincidence site lattice (CSL) displacement shift complete (DSC) lattice construction. The atomic arrangement in a perfect crystal is determined by the minimum of free energy and any deviation of the former from ideal positions inevitably causes an increase of the latter []. Consequently, it is safe to assume that the atoms will remain close to their ideal position. At certain misorientations between two crystallites, crystallographic planes exist that transcend the grain boundary from one crystallite to the other, i. e. certain atomic positions in the grain boundary coincide with ideal positions in both neighboring crystallites. These atomic positions are termed coincidence sites and the super lattice containing these sites on the other hand is the aforementioned coincidence site lattice (CSL). The elementary cell of the CSL is selfevidently larger than the elementary cell of the crystal lattice and its volume may be calculated in terms of the lattice parameters of the crystal lattice. The CSL is characterized by the density of its coincidence sites, which in turn are defined by the quantity []: volume of elementary cell CSL (.6) volume of elementary cell of crystal lattice Since coincidence sites are representations of atoms located at ideal fit positions, it is safe to assume that grain boundaries preferably stretch along coincidence sites []. 1
10 a 5a 5 a a DSC latticedsc CSL CSL CSL CSL a a lattice point grain I a) lattice point grain II b) Fig. 15: a) Coincidence site lattice (CSL) of a <100> grain boundary (=5). Left: grain boundary plane is perpendicular to paper plane (tilt boundary). Right: grain boundary plane is parallel to paper plane (twist boundary). b) CSL and displacement shift complete lattice (DSC) at <100> rotation in a cubic lattice. [1] Grain boundaries containing a high density of coincidence sites are called CSL boundaries or special boundaries. The order of the boundary increases with the decrease of the value, which is always an odd integer. Experimental data show that CSL grain boundaries of low indeed consist of a low energy configuration, which is reflected by a low free surface energy [10, 11] and low grain boundary migration activation enthalpy [1]. However, there is a fundamental problem in applying this concept to real, arbitrary grain boundaries: since the CSL only exists at very special, defined angles and does not continually change with misorientation angle, the long range coincidence is lost even for small deviations []. This may be compensated by the introduction of dislocations with DSC Burgers vectors which are also referred to as 13
11 secondary grain boundary dislocations (SGBDs), as they are confined to the grain boundary [1]. Detailed analysis revealed that 7 different polyhedra (see. Fig. 16) are necessary to account for all possible arrangements of atoms in a grain boundary [13]. () () () () () Fig. 16: () () The seven Bernal structures, of which the structural units of GBs are composed [13, 38]. These polyhedra represent characteristic structures of the grain boundary and are thus termed structural units. It has been shown by computer simulations, that low energy boundaries consist of only one type of structural unit []. Upon changing the orientation relationship, other structural units are introduced into the boundary plane, which are identical to the cores of SGBDs. The density of the newly introduced structural units increases with the grain boundaries misorientation angle, until eventually the grain boundary structure solely 14
12 consists of these new structural units. This concept of structural units constitutes our current understanding of grain boundary structures [1]. Analogously to the dislocation model of LAGBs, where the model by Read and Shockley [6] applies, the CSLDSC model is no longer valid above a maximum deviation from exact CSLmisorientations, because the spacing of the SGBDs decreases with increasing deviation. As such, the SGBDs above a certain deviation of the misorientation angle tend to overlap and therefore lose their individuality. The most common criterion for the maximum deviation proposed by Brandon [15] reads: 15 (7) Grain boundaries satisfying this criterion are referred to as special grain boundaries as opposed to random grain boundaries Classical model of grain boundary motion Over the past 60 years, grain boundary motion has been subjected to extensive experimental and theoretical investigations. However, to this day no unified theory about grain boundary migration has been published, which were able to account for phenomena such as the misorientation dependence of grain boundary mobility as observed for instance by Aust and Rutter [16]. Basically, all theoretical attempts to describe grain boundary motion are based on the reaction rate theory by Smoluchoski [17] and Turnbull et al. [18], in which individual atoms cross the grain boundary accompanied by a net energy gain. It 15
13 is assumed that the detachment of one atom from a crystal to join the crystal across the boundary destroys a lattice site rather than creating a vacancy and that its attachment to the adjacent crystal surface generates a new lattice site as opposed to eliminating a vacancy [1]. G Grain boundary Grain 1 Grain free energy G G m Pb p 3 G m x Fig. 17: The free energy G of a moving atom changes by the driving force pb 3 when it crosses the grain boundary. G m is the free energy barrier for bulk diffusion [1]. Following these assumptions, grain boundary motion is conveniently simplified to diffusive motion of single atoms across the boundary rather than the uniform motion of atom groups. We shall now derive the rate equation for grain boundary velocity, as seen in Ref. [1]: for the simplest case, the grain boundary is assumed to have a thickness of a monatomic layer, hence the boundary may be crossed by a single atomic jump and each transferred atom displaces the boundary by the diameter of an atom. Grain boundary velocity v is then expressed by [19] 16
14 v b (.8) where + and  are the jump frequencies in opposite directions, respectively. In case of zero difference in Gibbs free energy between the two grains, the net flux will also equal zero. However, any difference in Gibbs free energy per unit volume gives rise to a driving force p: dg p (.9) dv In that case, each atom attaching to the growing grain of volume 3 b 3 will gain the energy 3 pb The change in Gibbs free energy associated with this process is schematically shown in Fig The grain boundary velocity then reads: 3 G m Gm pb v b exp exp (.10) kt kt The assumption of equal jump frequencies + =  = D ( D Debyefrequency) and equal migration free energy G m for both jump directions simplifies the equation to 3 G m pb v b D exp 1 exp kt (.11) kt 17
15 Further assuming that pb 3 <<kt for T 0.3T m, a series expansion of the second exponential term 3 3 pb pb exp 1 (.1) kt kt finally yields for velocity v b vd G exp m kt kt v 4 p m p (.13) where m is referred to as grain boundary mobility, the proportionality factor of the fundamental linear relationship between grain boundary velocity and driving force. Variable m basically contains all the kinetic characteristics of the grain boundary. Furthermore, it is also distinguished between the intrinsic mobility determined by grain boundary misorientation and inclination and the extrinsic mobility primarily governed by impurity content and dislocation densities. By introducing the NernstEinstein relation for general diffusive processes (volume diffusion, grain boundary diffusion, etc.) without specification into the equation, the relation between grain boundary mobility and diffusion of atoms across the boundary reads: b D m m m0 exp kt H kt (.14) 18
16 D m is the diffusion coefficient for diffusion jumps through the boundary, m 0 and H are the preexponential factor and activation enthalpy of the grain boundary mobility. This simple model may be modified by assuming the detachments to occur in a sequence of steps or thermal grain boundary vacancies to assist diffusion [0]. However, these modifications will only affect the preexponential factor m 0 and the activation enthalpy H of mobility m leaving the migration rate v and the driving force p unaffected [1] Driving forces of grain boundary migration The driving force p is a force acting per unit area on a grain boundary and its source may be of various origins. Generally, a driving force emerges when the motion of a grain boundary results in reducing the system s overall free energy. A gradient of any intensive thermodynamic variable offers a source of such driving forces: temperature gradients, pressure, density of defects, energy density (elastic, magnetic, electrical), etc. A more detailed treatise on the various driving forces utilized in grain boundary migration experiments was written by Gottstein and Shvindlerman [1] Magnetic driving force We shall now take a detailed look at the magnetic driving force, which was predominantly applied to induce grain boundary migration in the experiments featured in this work. Mullins was the first to use the driving force induced by a 19
17 high magnetic field to induce grain boundary migration in bismuth polycrystals [1]. Due to its anisotropic properties, zinc possesses a different magnetic susceptibility parallel ( II ) and perpendicular ( ) to its hexagonal or caxis such that II >. The susceptibility tensor is represented by: (.15) 0 0 As shown schematically in Fig. 18 below, the susceptibility tensor surface for zinc has an ellipsoidal shape. Therefore, inside a magnetic field a driving force for grain boundary motion is induced between two crystallites due to a difference of magnetic free energy density, which is given by H 0 H H M dh 1 l l 0 0 ij i j (.16) where 0 is the vacuum permeability and H is the magnetic field strength. The magnetic polarization specific to the material is given by M H (see eq..15) and l s = cos s are the cosines between the principal crystal axes and the magnetic field H. 0
18 c H a 3 H a 1 a Fig. 18: Schematic depiction of the anisotropy of magnetic susceptibility in zinc, with respect to the unit cell. The spatial dependence of the magnetic susceptibility may be described by a second rank tensor and is represented by an ellipsoidal surface []. As shown analogously in Ref. [] for other anisotropic crystal properties, we shall in the following develop a general expression for the magnetic driving force. Taking into account, that there are only two independent susceptibility components in zinc, equation.16 reduces to: H 0 1 l1 l3 l (.17) which since 1 l l3 l1 l 1 l 3 1 l (.18) may be further simplified to: 1
19 H cos 3 (.19) Thus, a general expression is obtained for the magnetic free energy density associated with a given orientation of a zinc crystal in an external magnetic field, dependent on only one spatial variable, 3, the angle between the crystallographic caxis and magnetic field vector H. To calculate the driving force for magnetically induced grain boundary motion p, the magnetic free energy density associated with the two orientations of the crystallites in the magnetic field separated by the grain boundary have to be subtracted from one another, which finally results in: p H 1 0 cos 1 cos (.0) where and 1 are the angles between the caxes in both neighboring crystallites and the magnetic field H. The susceptibility difference in Zn was measured to be = and found not to depend on the temperature [3]. Now that the driving force for bicrystalline samples was deduced, we will proceed to magnetic driving forces in polycrystals: as applied in [4, 5], the magnetic driving force for the growth of each grain in a polycrystal is given by equation.1 below. Like discussed above for the case of bicrystalline samples, the crystallites with energetically favorable caxis orientation with respect to the field are bound to grow while the crystallite with a less favorable orientation
20 will shrink. This is caused by the differing magnetic susceptibility in zinc parallel and perpendicular to its crystallographic caxis. Equation.1, as introduced in Ref. [4], describes the magnetic driving force acting on one grain in a polycrystal, p m 0H 1 n j n j 1 0H cos n j cos n j (.1) where and j are the angles between field direction and the principal axes of the grain considered and its n neighboring grains. If 0 (which is true for Zn) and the condition cos 1/ n cos 0 n n is met by the one grain and its adjacent grains, the magnetic energy density in the one grain is lower than the average energy density of its neighboring grains ( ). Thus, the magnetic driving force promotes growth of the former grain, as then p m 0 [4]. The largest obtainable driving force is governed by the magnetic field strength at disposal and the magnetic susceptibility difference of the material under investigation. In the case of zinc, the maximum driving force p m is calculated to 1. kj/m 3 in high field magnets with a maximum field strength of 5 Tesla. Considering the applicability for grain boundary migration experiments, two major advantages over the capillary driving force (see section 1.6. below) are: 3
21 1.) The magnetic driving force facilitates the addressing of absolute grain boundary mobility as opposed to reduced mobility, thus enabling the migration measurements of crystallographically defined grain boundaries and studying the inclination dependence of activation parameters..) The possibility to adjust the magnitude of the driving force during the experiment. Curvature driven migration experiments do not yield the absolute mobility as a result, as the grain boundary inclination changes along the curvature and with it, consequently, its structure. Therefore, in curvature driven migration experiments one basically obtains the averaged mobility of a large set of differently inclined grain boundaries, rather than the absolute mobility of one spatially defined, planar boundary Capillary driving force Unlike with grain growth induced by a magnetic driving force, where the free energy gain during grain boundary motion originates from the alignment of crystal volume swept by the boundary to an orientation associated with lower magnetic susceptibility, the capillary driving force is provided by the free energy of the grain boundary and stems from the pressure difference p, caused by the difference of capillary forces on both sides of a curved grain boundary [1]. The capillary pressure is expressed by: 4
22 p 1 1 R1 R (.) where is the grain boundary free energy and R 1, R are the main radii of curvature under the assumption of boundary isotropy. Upon thermal activation this driving force induces boundary motion in the direction towards the center of curvature, causing a reduction of grain boundary area and, consequently, energy. However, the use of the capillary driving force only permits to evaluate a reduced boundary mobility, A m, where the grain boundary free energy is still part of the equation and thus factors into the obtained mobility values. 5
Defects Introduction. Bonding + Structure + Defects. Properties
Defects Introduction Bonding + Structure + Defects Properties The processing determines the defects Composition Bonding type Structure of Crystalline Processing factors Defects Microstructure Types of
More informationChapter Outline Dislocations and Strengthening Mechanisms
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
More informationCrystals are solids in which the atoms are regularly arranged with respect to one another.
Crystalline structures. Basic concepts Crystals are solids in which the atoms are regularly arranged with respect to one another. This regularity of arrangement can be described in terms of symmetry elements.
More informationChapter Outline Dislocations and Strengthening Mechanisms
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
More informationChapter Outline. How do atoms arrange themselves to form solids?
Chapter Outline How do atoms arrange themselves to form solids? Fundamental concepts and language Unit cells Crystal structures Simple cubic Facecentered cubic Bodycentered cubic Hexagonal closepacked
More informationChapter 7: Polarization
Chapter 7: Polarization Joaquín Bernal Méndez Group 4 1 Index Introduction Polarization Vector The Electric Displacement Vector Constitutive Laws: Linear Dielectrics Energy in Dielectric Systems Forces
More informationCHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS
71 CHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 The dislocation density is just the total dislocation length
More informationChapter Outline. Diffusion  how do atoms move through solids?
Chapter Outline iffusion  how do atoms move through solids? iffusion mechanisms Vacancy diffusion Interstitial diffusion Impurities The mathematics of diffusion Steadystate diffusion (Fick s first law)
More informationSolid State Device Fundamentals
Solid State Device Fundamentals ENS 345 Lecture Course by Alexander M. Zaitsev alexander.zaitsev@csi.cuny.edu Tel: 718 982 2812 Office 4N101b 1 Solids Three types of solids, classified according to atomic
More informationPlate waves in phononic crystals slabs
Acoustics 8 Paris Plate waves in phononic crystals slabs J.J. Chen and B. Bonello CNRS and Paris VI University, INSP  14 rue de Lourmel, 7515 Paris, France chen99nju@gmail.com 41 Acoustics 8 Paris We
More informationMaterial Deformations. Academic Resource Center
Material Deformations Academic Resource Center Agenda Origin of deformations Deformations & dislocations Dislocation motion Slip systems Stresses involved with deformation Deformation by twinning Origin
More informationPiezo Technologies  Technical Resource Paper
in Piezoceramic Materials One can think of a piezoceramic as a rock which generates electrical current if squeezed and which moves if driven by an electrical current. For these wonderful properties to
More information(10 4 mm 2 )(1000 mm 3 ) = 10 7 mm = 10 4 m = 6.2 mi
14:440:407 Fall 010 Additional problems and SOLUTION OF HOMEWORK 07 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 To provide
More information11.1. Objectives. Component Form of a Vector. Component Form of a Vector. Component Form of a Vector. Vectors and the Geometry of Space
11 Vectors and the Geometry of Space 11.1 Vectors in the Plane Copyright Cengage Learning. All rights reserved. Copyright Cengage Learning. All rights reserved. 2 Objectives! Write the component form of
More informationPhysics 9e/Cutnell. correlated to the. College Board AP Physics 1 Course Objectives
Physics 9e/Cutnell correlated to the College Board AP Physics 1 Course Objectives Big Idea 1: Objects and systems have properties such as mass and charge. Systems may have internal structure. Enduring
More informationImperfections in atomic arrangements
MME131: Lecture 8 Imperfections in atomic arrangements Part 1: 0D Defects A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Occurrence and importance of crystal defects Classification
More informationSolving Simultaneous Equations and Matrices
Solving Simultaneous Equations and Matrices The following represents a systematic investigation for the steps used to solve two simultaneous linear equations in two unknowns. The motivation for considering
More informationAjit Kumar Patra (Autor) Crystal structure, anisotropy and spin reorientation transition of highly coercive, epitaxial PrCo films
Ajit Kumar Patra (Autor) Crystal structure, anisotropy and spin reorientation transition of highly coercive, epitaxial PrCo films https://cuvillier.de/de/shop/publications/1306 Copyright: Cuvillier Verlag,
More informationLecture 2. Surface Structure
Lecture 2 Surface Structure Quantitative Description of Surface Structure clean metal surfaces adsorbated covered and reconstructed surfaces electronic and geometrical structure References: 1) Zangwill,
More informationHow is a vector rotated?
How is a vector rotated? V. Balakrishnan Department of Physics, Indian Institute of Technology, Madras 600 036 Appeared in Resonance, Vol. 4, No. 10, pp. 6168 (1999) Introduction In an earlier series
More informationBasic Concepts of Crystallography
Basic Concepts of Crystallography Language of Crystallography: Real Space Combination of local (point) symmetry elements, which include angular rotation, centersymmetric inversion, and reflection in mirror
More informationReciprocal Space and Brillouin Zones in Two and Three Dimensions As briefly stated at the end of the first section, Bloch s theorem has the following
Reciprocal Space and Brillouin Zones in Two and Three Dimensions As briefly stated at the end of the first section, Bloch s theorem has the following form in two and three dimensions: k (r + R) = e 2 ik
More informationk u (t) = k b + k s t
Chapter 2 Stripe domains in thin films 2.1 Films with perpendicular anisotropy In the first part of this chapter, we discuss the magnetization of films with perpendicular uniaxial anisotropy. The easy
More informationThe atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
More informationChapter 5: Diffusion. 5.1 SteadyState Diffusion
: Diffusion Diffusion: the movement of particles in a solid from an area of high concentration to an area of low concentration, resulting in the uniform distribution of the substance Diffusion is process
More informationMaterials Science and Engineering Department MSE , Sample Test #1, Spring 2010
Materials Science and Engineering Department MSE 200001, Sample Test #1, Spring 2010 ID number First letter of your last name: Name: No notes, books, or information stored in calculator memories may be
More informationCHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS
41 CHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS Vacancies and SelfInterstitials 4.1 In order to compute the fraction of atom sites that are vacant in copper at 1357 K, we must employ Equation
More informationv kt = N A ρ Au exp (
42 4.2 Determination of the number of vacancies per cubic meter in gold at 900 C (1173 K) requires the utilization of Equations 4.1 and 4.2 as follows: N v N exp Q v N A ρ Au kt A Au exp Q v kt (6.023
More informationDeformation of Single Crystals
Deformation of Single Crystals When a single crystal is deformed under a tensile stress, it is observed that plastic deformation occurs by slip on well defined parallel crystal planes. Sections of the
More informationLECTURE SUMMARY September 30th 2009
LECTURE SUMMARY September 30 th 2009 Key Lecture Topics Crystal Structures in Relation to Slip Systems Resolved Shear Stress Using a Stereographic Projection to Determine the Active Slip System Slip Planes
More informationNEW YORK STATE TEACHER CERTIFICATION EXAMINATIONS
NEW YORK STATE TEACHER CERTIFICATION EXAMINATIONS TEST DESIGN AND FRAMEWORK September 2014 Authorized for Distribution by the New York State Education Department This test design and framework document
More informationIntroduction To Materials Science FOR ENGINEERS, Ch. 5. Diffusion. MSE 201 Callister Chapter 5
Diffusion MSE 21 Callister Chapter 5 1 Goals: Diffusion  how do atoms move through solids? Fundamental concepts and language Diffusion mechanisms Vacancy diffusion Interstitial diffusion Impurities Diffusion
More informationME 612 Metal Forming and Theory of Plasticity. 1. Introduction
Metal Forming and Theory of Plasticity Yrd.Doç. e mail: azsenalp@gyte.edu.tr Makine Mühendisliği Bölümü Gebze Yüksek Teknoloji Enstitüsü In general, it is possible to evaluate metal forming operations
More informationBCM 6200  Protein crystallography  I. Crystal symmetry Xray diffraction Protein crystallization Xray sources SAXS
BCM 6200  Protein crystallography  I Crystal symmetry Xray diffraction Protein crystallization Xray sources SAXS Elastic Xray Scattering From classical electrodynamics, the electric field of the electromagnetic
More informationState of Stress at Point
State of Stress at Point Einstein Notation The basic idea of Einstein notation is that a covector and a vector can form a scalar: This is typically written as an explicit sum: According to this convention,
More informationStructure Factors 59553 78
78 Structure Factors Until now, we have only typically considered reflections arising from planes in a hypothetical lattice containing one atom in the asymmetric unit. In practice we will generally deal
More informationFigure 1.1 Vector A and Vector F
CHAPTER I VECTOR QUANTITIES Quantities are anything which can be measured, and stated with number. Quantities in physics are divided into two types; scalar and vector quantities. Scalar quantities have
More informationBasics in Xray Diffraction and Special Application
Basics in Xray Diffraction and Special Application Introduction: Xray Diffraction (XRD) helps one to reach the science at atomic scale in the analysis of crystal structure, chemical composition, and
More informationMAE 20 Winter 2011 Assignment 3 solutions
MAE 20 Winter 2011 Assignment 3 solutions 4.3 Calculate the activation energy for vacancy formation in aluminum, given that the equilibrium number of vacancies at 500 C (773 K) is 7.57 10 23 m 3. The
More informationLecture 4: Thermodynamics of Diffusion: Spinodals
Materials Science & Metallurgy Master of Philosophy, Materials Modelling, Course MP6, Kinetics and Microstructure Modelling, H. K. D. H. Bhadeshia Lecture 4: Thermodynamics of Diffusion: Spinodals Fick
More informationUniversity of Cambridge, Materials Science & Metallurgy. Dilatometry
University of Cambridge, Materials Science & Metallurgy H. K. D. H. Bhadeshia Dilatometry The dilatometric method utilises either transformation strains or thermal strains; the basic data generated are
More informationAdvanced Lab Course. MOKE Microscopy
Advanced Lab Course MOKE Microscopy M209 Stand: 20160408 Aim: Characterization of magnetization reversal of magnetic bulk and thin film samples by means of magnetooptical Kerr effect and recording of
More informationEðlisfræði 2, vor 2007
[ Assignment View ] [ Pri Eðlisfræði 2, vor 2007 28. Sources of Magnetic Field Assignment is due at 2:00am on Wednesday, March 7, 2007 Credit for problems submitted late will decrease to 0% after the deadline
More informationCh. 4: Imperfections in Solids Part 1. Dr. Feras Fraige
Ch. 4: Imperfections in Solids Part 1 Dr. Feras Fraige Outline Defects in Solids 0D, Point defects vacancies Interstitials impurities, weight and atomic composition 1D, Dislocations edge screw 2D, Grain
More informationPSS 27.2 The Electric Field of a Continuous Distribution of Charge
Chapter 27 Solutions PSS 27.2 The Electric Field of a Continuous Distribution of Charge Description: Knight ProblemSolving Strategy 27.2 The Electric Field of a Continuous Distribution of Charge is illustrated.
More informationCHAPTER 3: CRYSTAL STRUCTURES
CHAPTER 3: CRYSTAL STRUCTURES Crystal Structure: Basic Definitions  lecture Calculation of material density selfprep. Crystal Systems lecture + selfprep. Introduction to Crystallography lecture + selfprep.
More informationChapter 3: The Structure of Crystalline Solids
Sapphire: cryst. Al 2 O 3 Insulin : The Structure of Crystalline Solids Crystal: a solid composed of atoms, ions, or molecules arranged in a pattern that is repeated in three dimensions A material in which
More information* Biot Savart s Law Statement, Proof Applications of Biot Savart s Law * Magnetic Field Intensity H * Divergence of B * Curl of B. PPT No.
* Biot Savart s Law Statement, Proof Applications of Biot Savart s Law * Magnetic Field Intensity H * Divergence of B * Curl of B PPT No. 17 Biot Savart s Law A straight infinitely long wire is carrying
More informationCrystal Symmetries METE 327 Physical Metallurgy Copyright 2008 Loren A. Jacobson 5/16/08
Crystal Symmetries Why should we be interested? Important physical properties depend on crystal structure Conductivity Magnetic properties Stiffness Strength These properties also often depend on crystal
More informationBoundary Conditions in Fluid Mechanics
Boundary Conditions in Fluid Mechanics R. Shankar Subramanian Department of Chemical and Biomolecular Engineering Clarkson University The governing equations for the velocity and pressure fields are partial
More informationConstitutive Equations  Plasticity
MCEN 5023/ASEN 5012 Chapter 9 Constitutive Equations  Plasticity Fall, 2006 1 Mechanical Properties of Materials: Modulus of Elasticity Tensile strength Yield Strength Compressive strength Hardness Impact
More information3. Diodes and Diode Circuits. 3. Diodes and Diode Circuits TLT8016 Basic Analog Circuits 2005/2006 1
3. Diodes and Diode Circuits 3. Diodes and Diode Circuits TLT8016 Basic Analog Circuits 2005/2006 1 3.1 Diode Characteristics SmallSignal Diodes Diode: a semiconductor device, which conduct the current
More informationslip lines which are close to, but not coincident with, the slip lines formed in
FATIGUE CRACK NUCLEATION IN AIETALS* BY T. II. LIN ANI) Y. A11. ITO UNIVERSITY OF CALIFORNIA (LOS ANGELES) Communicated by T'. Y. Thomas, December 18, 1968 Abstract. One of the unanswered questions in
More informationGeometrical symmetry and the fine structure of regular polyhedra
Geometrical symmetry and the fine structure of regular polyhedra Bill Casselman Department of Mathematics University of B.C. cass@math.ubc.ca We shall be concerned with geometrical figures with a high
More informationCrystal Defects p. 2. Point Defects: Vacancies. Department of Materials Science and Engineering University of Virginia. Lecturer: Leonid V.
Crystal Defects p. 1 A twodimensional representation of a perfect single crystal with regular arrangement of atoms. But nothing is perfect, and structures of real materials can be better represented by
More informationDifferential Relations for Fluid Flow. Acceleration field of a fluid. The differential equation of mass conservation
Differential Relations for Fluid Flow In this approach, we apply our four basic conservation laws to an infinitesimally small control volume. The differential approach provides point by point details of
More informationCHAPTER 3 THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS
CHAPTER THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS Fundamental Concepts.6 Show that the atomic packing factor for HCP is 0.74. The APF is just the total sphere volumeunit cell volume ratio.
More information" {h k l } lop x odl. ORxOS. (2) Determine the interplanar angle between these two planes:
Textures and Microstructures, 1991, Vols 1418, pp. 273278 Reprints available from the publisher Photocopying permitted by license only (C) 1991 Gordon and Breach Science Publishers SA Printed in the
More informationRelevant Reading for this Lecture... Pages 8387.
LECTURE #06 Chapter 3: Xray Diffraction and Crystal Structure Determination Learning Objectives To describe crystals in terms of the stacking of planes. How to use a dot product to solve for the angles
More informationNotes on Elastic and Inelastic Collisions
Notes on Elastic and Inelastic Collisions In any collision of 2 bodies, their net momentus conserved. That is, the net momentum vector of the bodies just after the collision is the same as it was just
More informationElasticity and Equations of State
Elasticity and Equations of State The way planets deform depends primarily upon the elastic properties of the constituent polycrystalline materials. In particular, the speed of body waves passing through
More informationThe First Law of Thermodynamics: Closed Systems. Heat Transfer
The First Law of Thermodynamics: Closed Systems The first law of thermodynamics can be simply stated as follows: during an interaction between a system and its surroundings, the amount of energy gained
More informationLecture 3 Fluid Dynamics and Balance Equa6ons for Reac6ng Flows
Lecture 3 Fluid Dynamics and Balance Equa6ons for Reac6ng Flows 3. 1 Basics: equations of continuum mechanics  balance equations for mass and momentum  balance equations for the energy and the chemical
More informationChapter 11 Equilibrium
11.1 The First Condition of Equilibrium The first condition of equilibrium deals with the forces that cause possible translations of a body. The simplest way to define the translational equilibrium of
More informationCurrent Standard: Mathematical Concepts and Applications Shape, Space, and Measurement Primary
Shape, Space, and Measurement Primary A student shall apply concepts of shape, space, and measurement to solve problems involving two and threedimensional shapes by demonstrating an understanding of:
More informationAlgebra 1 2008. Academic Content Standards Grade Eight and Grade Nine Ohio. Grade Eight. Number, Number Sense and Operations Standard
Academic Content Standards Grade Eight and Grade Nine Ohio Algebra 1 2008 Grade Eight STANDARDS Number, Number Sense and Operations Standard Number and Number Systems 1. Use scientific notation to express
More informationCORRELATED TO THE SOUTH CAROLINA COLLEGE AND CAREERREADY FOUNDATIONS IN ALGEBRA
We Can Early Learning Curriculum PreK Grades 8 12 INSIDE ALGEBRA, GRADES 8 12 CORRELATED TO THE SOUTH CAROLINA COLLEGE AND CAREERREADY FOUNDATIONS IN ALGEBRA April 2016 www.voyagersopris.com Mathematical
More informationA Theoretical Model for Mutual Interaction between Coaxial Cylindrical Coils Lukas Heinzle
A Theoretical Model for Mutual Interaction between Coaxial Cylindrical Coils Lukas Heinzle Page 1 of 15 Abstract: The wireless power transfer link between two coils is determined by the properties of the
More informationRef. Ch. 11 in Superalloys II Ch. 8 in Khanna Ch. 14 in Tien & Caulfield
MTE 585 Oxidation of Materials Part 1 Ref. Ch. 11 in Superalloys II Ch. 8 in Khanna Ch. 14 in Tien & Caulfield Introduction To illustrate the case of high temperature oxidation, we will use Nibase superalloys.
More informationNEW MEXICO Grade 6 MATHEMATICS STANDARDS
PROCESS STANDARDS To help New Mexico students achieve the Content Standards enumerated below, teachers are encouraged to base instruction on the following Process Standards: Problem Solving Build new mathematical
More informationFURTHER VECTORS (MEI)
Mathematics Revision Guides Further Vectors (MEI) (column notation) Page of MK HOME TUITION Mathematics Revision Guides Level: AS / A Level  MEI OCR MEI: C FURTHER VECTORS (MEI) Version : Date: 97 Mathematics
More informationσ = F / A o Chapter Outline Introduction Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? and Tension Compression Shear Torsion Elastic deformation Chapter Outline Introduction To understand and describe how materials
More informationINSTITUTE FOR APPLIED PHYSICS Physical Practice for Learners of Engineering sciences Hamburg University, Jungiusstraße 11
INSTITUTE FOR APPIED PHYSICS Physical Practice for earners of Engineering sciences Hamburg University, Jungiusstraße 11 Hall effect 1 Goal Characteristic data of a test semiconductor (Germanium) should
More informationCoefficient of Potential and Capacitance
Coefficient of Potential and Capacitance Lecture 12: Electromagnetic Theory Professor D. K. Ghosh, Physics Department, I.I.T., Bombay We know that inside a conductor there is no electric field and that
More informationThe Kinetic Theory of Gases Sections Covered in the Text: Chapter 18
The Kinetic Theory of Gases Sections Covered in the Text: Chapter 18 In Note 15 we reviewed macroscopic properties of matter, in particular, temperature and pressure. Here we see how the temperature and
More information14:635:407:02 Homework III Solutions
14:635:407:0 Homework III Solutions 4.1 Calculate the fraction of atom sites that are vacant for lead at its melting temperature of 37 C (600 K). Assume an energy for vacancy formation of 0.55 ev/atom.
More informationPIEZO CERAMICS. Noliac Group develops and manufactures piezoelectric. zirconate titanate (PZT) of high quality and tailored for custom
Noliac Group develops and manufactures piezoelectric zirconate titanate (PZT) of high quality and tailored for custom Piezoelectric components may be used as e.g.: Actuators Sensors Generators Transducers
More informationTWODIMENSIONAL XRAY DIFFRACTION
TWODIMENSIONAL XRAY DIFFRACTION BOB B. HE GQ WILEY ,. "'! :~! CONTENTS~\..~..). Preface 1. Introduction 1.1 XRay Technology and Its Brief History, 1.2 Geometry of Crystals, 2 1.2.1 Crystal Lattice
More informationTwo vectors are equal if they have the same length and direction. They do not
Vectors define vectors Some physical quantities, such as temperature, length, and mass, can be specified by a single number called a scalar. Other physical quantities, such as force and velocity, must
More informationWhen the fluid velocity is zero, called the hydrostatic condition, the pressure variation is due only to the weight of the fluid.
Fluid Statics When the fluid velocity is zero, called the hydrostatic condition, the pressure variation is due only to the weight of the fluid. Consider a small wedge of fluid at rest of size Δx, Δz, Δs
More informationChapter Outline. Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility
More informationThe Role of Electric Polarization in Nonlinear optics
The Role of Electric Polarization in Nonlinear optics Sumith Doluweera Department of Physics University of Cincinnati Cincinnati, Ohio 45221 Abstract Nonlinear optics became a very active field of research
More informationIntroduction of LDA. Last Class: 1. Matlab Programming 2. An example of PIV in Matlab code 3. EDPIV 4. PIV plugin for ImageJ 5.
Introduction of LDA Last Class: 1. Matlab Programming 2. An example of PIV in Matlab code 3. EDPIV 4. PIV plugin for ImageJ 5. JPIV Today s Contents: 1. Fundamentals of LDA 2. Turbulent Flow Properties
More informationSouth Carolina College and CareerReady (SCCCR) PreCalculus
South Carolina College and CareerReady (SCCCR) PreCalculus Key Concepts Arithmetic with Polynomials and Rational Expressions PC.AAPR.2 PC.AAPR.3 PC.AAPR.4 PC.AAPR.5 PC.AAPR.6 PC.AAPR.7 Standards Know
More informationAP Physics C Chapter 23 Notes Yockers Faraday s Law, Inductance, and Maxwell s Equations
AP Physics C Chapter 3 Notes Yockers Faraday s aw, Inductance, and Maxwell s Equations Faraday s aw of Induction  induced current a metal wire moved in a uniform magnetic field  the charges (electrons)
More information6 J  vector electric current density (A/m2 )
Determination of Antenna Radiation Fields Using Potential Functions Sources of Antenna Radiation Fields 6 J  vector electric current density (A/m2 ) M  vector magnetic current density (V/m 2 ) Some problems
More informationMechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied
Mechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied Stress and strain fracture or engineering point of view: allows to predict the
More informationCrystal Structure Determination I
Crystal Structure Determination I Dr. Falak Sher Pakistan Institute of Engineering and Applied Sciences National Workshop on Crystal Structure Determination using Powder XRD, organized by the Khwarzimic
More informationMartensite in Steels
Materials Science & Metallurgy http://www.msm.cam.ac.uk/phasetrans/2002/martensite.html H. K. D. H. Bhadeshia Martensite in Steels The name martensite is after the German scientist Martens. It was used
More informationStress Analysis, Strain Analysis, and Shearing of Soils
C H A P T E R 4 Stress Analysis, Strain Analysis, and Shearing of Soils Ut tensio sic vis (strains and stresses are related linearly). Robert Hooke So I think we really have to, first, make some new kind
More informationNotes: Most of the material presented in this chapter is taken from Bunker and Jensen (2005), Chap. 3, and Atkins and Friedman, Chap. 5.
Chapter 5. Geometrical ymmetry Notes: Most of the material presented in this chapter is taken from Bunker and Jensen (005), Chap., and Atkins and Friedman, Chap. 5. 5.1 ymmetry Operations We have already
More informationThe Viscosity of Fluids
Experiment #11 The Viscosity of Fluids References: 1. Your first year physics textbook. 2. D. Tabor, Gases, Liquids and Solids: and Other States of Matter (Cambridge Press, 1991). 3. J.R. Van Wazer et
More informationPhysics 53. Rotational Motion 1. We're going to turn this team around 360 degrees. Jason Kidd
Physics 53 Rotational Motion 1 We're going to turn this team around 360 degrees. Jason Kidd Rigid bodies To a good approximation, a solid object behaves like a perfectly rigid body, in which each particle
More informationXray thinfilm measurement techniques
Technical articles Xray thinfilm measurement techniques II. Outofplane diffraction measurements Toru Mitsunaga* 1. Introduction A thinfilm sample is twodimensionally formed on the surface of a substrate,
More informationModern Construction Materials Prof. Ravindra Gettu Department of Civil Engineering Indian Institute of Technology, Madras
Modern Construction Materials Prof. Ravindra Gettu Department of Civil Engineering Indian Institute of Technology, Madras Module  2 Lecture  2 Part 2 of 2 Review of Atomic Bonding II We will continue
More informationModule #17. Work/Strain Hardening. READING LIST DIETER: Ch. 4, pp. 138143; Ch. 6 in Dieter
Module #17 Work/Strain Hardening READING LIST DIETER: Ch. 4, pp. 138143; Ch. 6 in Dieter D. KuhlmannWilsdorf, Trans. AIME, v. 224 (1962) pp. 10471061 Work Hardening RECALL: During plastic deformation,
More informationStructural Integrity Analysis
Structural Integrity Analysis 1. STRESS CONCENTRATION Igor Kokcharov 1.1 STRESSES AND CONCENTRATORS 1.1.1 Stress An applied external force F causes inner forces in the carrying structure. Inner forces
More informationCommon Core State Standards for Mathematics Accelerated 7th Grade
A Correlation of 2013 To the to the Introduction This document demonstrates how Mathematics Accelerated Grade 7, 2013, meets the. Correlation references are to the pages within the Student Edition. Meeting
More informationSome Comments on the Derivative of a Vector with applications to angular momentum and curvature. E. L. Lady (October 18, 2000)
Some Comments on the Derivative of a Vector with applications to angular momentum and curvature E. L. Lady (October 18, 2000) Finding the formula in polar coordinates for the angular momentum of a moving
More informationInteractive Math Glossary Terms and Definitions
Terms and Definitions Absolute Value the magnitude of a number, or the distance from 0 on a real number line Additive Property of Area the process of finding an the area of a shape by totaling the areas
More information